# x 45 matrix was machine diagonalised and exact agreement was obtained.

In document Optical studies of off-centre ions in strontium oxide (Page 131-136)

5.7 Discussion of the Crystal Field Parameters

The problem is to parameterize the four strong bands observed in the experiment at 19000, 15800, 13500 and 6000 cm ^ . The results of

2 8

a d ’ cubic field calculation are reproduced in Figure 5.1 from

reference . For the present case spin-orbit, B, and C have not been used as entirely free parameters, rather they have been given values

2+ slightly lower than the free ion values for Ni

Calculation of selection rules for C„ 3Ä2 3Ä2 and 3A2 3E 3v

electric dipole transitions have been made using the coupling coefficients of Koster (see Appendix I ) . The results are summarised for the infra-red band in Figure 5.2. It means that a 3A2 -*■ 3A£ will only give one strong tt transition from

the T3 component of the ground state (the Greek script denotes the spin-orbit component of the trigonal term). This is the observed

situation for the 13500 cm ^ band and consequently the line is assigned to ^ 2(^3) -> 3A2( E 3) transition.

B = 610 cm-1 C = 2500 cm ^ v = 800 cm C = 155 cm-1

The calculation also suggests that transitions from the T3 component of the ground state should give three lines with the symmetry of the excited state being T^, T2 and T3 belonging to a 3E trigonal level.

This is exactly what is observed in the 6000 cm ^ band. Furthermore,

the hot band possibly to an T3 level is also produced in the model. So

the components of the spin-orbit split °E are all located.

With the above assignments it is possible to select two values of Dq, about -600 cm ^ and -320 cm \ which give rise to spin-allowed

bands at 6000 and 13500 cm \ In the first model (A) they would arise

from trigonally split components of the dTi term, whereas in the second model (B) the infra-red band arises from this term and the strong bands

o b

in the visible would have their origin in the Tj term.

There are, however, a number of indications that model B with the lower cubic field parameter is actually the correct physical

situation. The splitting of the 3T t e r m into the 3E and 3Ä trigonal

components varies as ~(v-v') and that of the 3T^a as ~(v+vT). To achieve

the observed energy level ordering with model A requires a large negative

v and positive v ’. However, such parameter values do not give the T3

component of JA2 as the ground state. Model B with a positive v gives

the correct order of ground state components and increasing the magnitude

of —v f reduces the ground state splitting. In addition, this model gives

the right ordering of the excited states.

The A level (at 15800 cm giving the rather weak band at

15800 cm ^ is not predicted, however, and is an outstanding difficulty, and remained so even when attempting to adjust the crystal field parameters in both minor and major ways (see Appendix II). We have not been able in any of these attempts to obtain a triplet level (S = 1) at this position while simultaneously fitting the other stronger bands (20000, 13500 and

75,000

I 5,000

10,000

Figure 5.1. Energy level curves for a d 8 electronic system immersed in

a field of octahedral symmetry for c = - 550 cm"1 , B = 950 cm"1 and C = 3150 cm"1 .

r 3 r 3 s+

### > ,|r'3

s_ > 4 3 s 0 >Ir 3 s 0 > Toll’s s+ > + -^lr3 T I^ 3 S+ " T ^ S

### |r2 s+ > , | r2

S > lr2 SO > (not observed) Ir2 s0 > lr2 s+ >>l s. > s s

### >

Figure 5.2. The selection rules for the infra-red band allowed

O A

transitions are indicated. All of the spin-orbit components are observed. The 'hot' line at 6408 cm ^ is not observed at low temperatures because it violates the spin-conservation rule (Am^ =0). The line observed at 4317 cm ^ might be due to the 3A2( r 3 ) -*•

### 3A2(r3)

transition. The spin-orbit functions are composed from the table of coupling coefficients in Appendix I.

6000) as triplets, i.e. spin allowed. The strength of the 15800 cm ^ indicates that it is more likely anyway to arise from a singlet level

and hence to be associated with a spin-forbidden transition. Familiarity

. 2+

with Ni spin-forbidden transitions in other systems would suggest that

this could arise from *E or the 1T2- However, of these the only T\ or T2 level is that associated with the 1T2* This state is split in

o b

similar fashion (order and magnitude) to the higher ^Tj band and hence

q * O b

always appears below the A2 component of the Tj which is claimed

to lie at 13500 cm . The spin-orbit splitting of the 3Ä2 itself, even

allowing for the interaction with this state, cannot displace by

1 O A

2300 cm from the '3A2(r'3) component (see Fig. 5.3). Further experiments

such as EPR/MCD double resonance seem desirable to conclusively establish that this band does indeed arise from the same centre.

An energy level diagram based on model B is shown in Figure 5.2 where D q , B, C and £ are fixed and the trigonal field components are

v ’ 1

varied in a fixed ratio — = - — and we see that the spin-allowed bands

are reasonably well predicted. It will be shown in the next section

(Part B) that a similar value of Dq is used to fit the spectrum of 2+

### m

* rH I

In document Optical studies of off-centre ions in strontium oxide (Page 131-136)